Reliability and Failure Analysis
of Electronic Components
By
Dr. Charles Surya, ENC
CD 636,
×
6220
ensurya@polyu.edu.hk
2
•
For VLSI Circuits to be a useful and growing technology, 2 conditions
must be satisfied:
–
Can be produced in large quantities at low cost
–
Cats can perform their functions throughout their intended lifetime
•
To lower the cost of manufacturing, one must determine the optimal
size of the IC.
•
The optimal size is a compromise between several competing
considerations:
–
Partitioning of the system
–
yield of good circuits
–
packaging and system assembly cost
–
reliability of complete system
•
Large number of IC’s results in high yield and assembly cost
•
To arrive at an optimal division of the system, we must be able to
predict the total system reliability as a function of the number of IC’s of
varying size
3
Mechanism of Yield Loss in VLSI
•
Cause for low yield falls into 3 basic categories:
–
Parametric processing problems
–
CKT design problems
–
random point defects in circuits
Processing Effects
•
Often a wafer is divided into regions good chips and bad chips (Fig. 1 p.
614, Sze)
•
This is most likely due to processing effects such as
–
Variations in thickness of oxide or polysilicon layers
–
Variations in resistance of implanted layers
–
Variations in width of lithographically defined features
4
•
Alignment of photomasks
–
e.g. PolySi gate lengths are shorter in thinner polySi regions than
in thicker polySi regions. This may cause channel lengths to be
too short and transistors cannot be turned off. This leads to
excessive leakage current
•
Variations in thickness of deposited dielectric lead to variations in
contact window size. This may lead to non

operative circuits if the
circuits depend on having a low value of contact resistance.
•
Variations in the doping of implanted layers which also leads to
variations in contact resistance
•
Also, wafer may vary in size during processing in excess of 20ppm.
Therefore a 125 mm wafer changes in size by 2.5mm. This may cause
significant misalignment.
5
Circuit Sensitivities
•
Certain areas of a wafer have low device yield because the design of a ckt
has failed to consider expected variations in device parameters and
correlation between variations in different parameters.
Point Defects
•
A 3
m dust can cause a break in a metal conductor
•
Si chunks may be knocked out of the wafer during processing
•
Isolated oxidation induced stacking fault may cause excessive leakage
current
Modeling of Yield

loss Mechanisms
•
We need to model IC yield in terms of fundamental parameters independent
of particular IC and characteristics of the process and processing line
because:
–
by accurately modeling the yield we can predict the cost and availability
of future ckts
6
–
once yield

modeling parameters are known one can compare
processing quality of different process lines and indicate where
improvements are required
•
IC yield is expressed as
Y=Y
0
Y
1
(D
0
,A,
i
)
•
1

Y
0
= fraction of bad chips due to processing related effects
1

Y
1
= remaining fraction of bad chips which is a function of
density of point defects
•
A is the chip area
•
i
is the parameter unique to different models of the yield
•
Y = ratio of good chips to total number of chips per wafer
•
All models predict Y decreases monotonically as A increases
•
Yield modeling can identify those processes and mechanisms that limit
yield of present IC
•
The process can then be improved or eliminated as needed
7
Uniform Density of Point Defects
•
In those areas where yield not degraded by either processing or ckt
sensitivities, the remaining cause of chip failure is randomly distributed
point defects (see See p. 617, 618)
•
A grid of 24 chip sites with 10 defects randomly distributed. In this
example 16 of the 24 sites have 0 defects
•
Of the remaining sites 6 have 1 defect no site has more than 2 defects
•
The problem of determining the yield is identical to the problem of placing
n balls in N cells and then calculating probability of a given cell containing
k balls
P
k
= (n!)/[k!(n

k)!]
(1)/(N
n
)(N

1)
n

k
•
If N and n are both large n/M = m remains finite and can be approximated
as
P
k
=e

m
m
k
/k!
•
The probability that a chip contains no defects is Y
1
= P
0
= e

m
•
The probability a chip contains 1 defect is
P
1
= me

m
8
•
If the area of the chip is A, the total chip area in the useable part of a
wafer is NA
•
The density of defects is n/NA = D
0
•
The average number of defects per chip, m, is m = n/N = D
0
NA/N = D
0
A
Y
1
= P
0
= exp(

D
0
A)
•
This Poisson estimation was used to predict yield in the early days in the
manufacture process
•
The actual yield was found to be much larger than predicted
9
Yield Enhancement using Redundant Circuitry
•
Many large MOS memory chips are designed with redundant circuitry,
which can be switched to replace defective circuit elements
•
This is usually accomplished using fusible links which can be fused as
needed using laser or other techniques
•
The yield will then be modified as shown
•
Y1 = P0 +
P
1
•
P0 = probability of chip containing no defects
•
P1 = probability of chip containing 1 defect
•
= probability of chip containing 1 defect and can be repaired by using a
single redundant column
Simple Non

uniform Distribution of D
•
Discrepancy between measured and predicted yield led to investigation of
non

uniform distribution of D
0
across a wafer
10
•
The yield can be expressed as
•
The yield is expressed as
Y =
exp(

DA) f(D) dD
•
f(D) is the normalized distribution of defect density
f(D) dD = 1
•
3 different D
0
are investigated:
–
Delta function Y
1
= exp(

D
0
A)
–
Triangular Y
2
= {[1

exp(

D
0
A)]/D
0
A}
2
–
Rectangular Y
3
= {1

exp(

2D
0
A)}/2D
0
A
•
for D
0
A >> 1 we find that
–
Y
1
= exp(

D
0
A)
–
Y
2
= 1/(D
0
A)
2
–
Y
3
= 1/(2D
0
A)
•
Y
3
is found to be most closely fit to the observed yield of large IC’s
•
The above distributions do not have any physical basis, therefore more
physically based distributions need to be investigated
11
Gamma Distribution
•
The Gamma distribution is more physical
f(D) = 1/[
(
)
(
)
]D

1
exp(

D/
)
•
and
are 2 distribution parameters and
(
) is the gamma function
•
Average density of defects =
•
Variance of D =
2
•
Consequently Y
4
= 1/(1+SD
0
A)
1/s
•
for s 0, Gamma function reduces to delta function and Y
4
exp(

D
0
A)
•
Using different values of s, Gamma function is a good approximations of
Y
2
and Y
3
over a wide range of D
0
A
•
Gamma yield functions can be used to represent a large variations in the
shape of experimental yield vs area curve see Fig. 4 and 5 p. 621 and 622
of Sze.
•
Each type of defect is characterized by
–
its mean defect density D
n0
–
shape factor of its distribution S
n
12
–
portion of total chip area A
n
susceptible that defect
–
Using Gamma yield function
Y
n
= 1/{(1+S
n
A
n
D
n0
)}
1/S
n
•
The overall yield is the product of the yield for each known type of defect
Y =
Y
n
for n=1,2,….,N
•
For a mature process in a well controlled high yield line, all of the major
yield

limiting defects have probably been controlled or eliminated. The
yield is a product of many terms each approximately 1.
•
This means S
n
A
n
D
n0
<< 1
ln Y =
[

(1/S
n
) ln(1+S
n
A
n
D
n0
)]
ln(1+S
n
A
n
D
n0
)
S
n
A
n
D
n0
Thus lnY =

A
n
D
n0
Y = exp(

A
n
D
n0
)
D* = (1/A)
A
n
D
n0
Y = exp(

AD*)
•
Here A
n
is the total chip area susceptible to the particular defect
13
Reliability Requirements for VLSI
•
It is instructive to consider examples of the effects of device failure
–
Early discrete solid state computer systems typically consisted of 10
5
transistors per system
–
If 1 device failure per month is set as the minimum acceptable
condition then the failure rate
< 1/(10
5
720 hrs)
= 14
10

9
failure/device

hour
•
1 FIT
1 failure/ 10
9
device

hour
•
The objective for the hypothetical system is for
< 14 FIT
Reliability Theory (Sze p. 627)
•
Useful mathematical description requires precise definition of the terms
•
Definitions:
–
Reliability

probability that an item will perform a
required
function
under
stated
conditions
for a
stated
period
of time
14
•
For an IC the
required
function
is generally defined by a test program for
an automatic test set
•
Often initial test programs are not complete and the ckts are not tested
under “all” required conditions
•
As new device failure modes are identified, the appropriate tests are
included in later test programs
•
Stated
Conditions

comprise of the total physical environments,
including mechanical, thermal, electrical ….
•
Stated
period
of
time

the time during which satisfactory operation is
required
Cumulative Distribution Function
•
If the device is operational at
t
= 0. The probability that the device will
fail at or before
t
is given by the function
F(t)
F(t) = 0
t < 0
0
F(t)
F(t`)
0
t
t`
F(t) 1
t
15
Reliability Function and Probability Density Function
•
The probability density function is
f(t) = dF(t)/dt
•
The Cumulative distribution function is
F(t) =
0
t
f(x)dx
•
The reliability function is
R(t) =
t
f (x)dx
•
Thus f(t) =

dR(t)/dt
16
Failure Rate
•
In many applications the quantity of most concern is the instantaneous
failure rate
•
This is often referred to as the hazard rate
•
Fraction of devices that were good at time t and that fail by t +
is
given by
•
F(t +
)

F(t) = R(t)

R(t+
)
•
The average failure rate during the time interval,
, is
•
(
t) = average failure rate
•
= 1/
[R(t)

R(t+
)]/R(t)
•
for
0
•
(t) =

1/R(t) dR(t)/dt = f(t)/R(t)
•
= f(t)/[1

F(t)]
•
=

d[ln R(t)]/dt
•
R(t) = exp[

0t
(x) dx]
17
Mean Time to Failure (MTTF)
and Common Distribution Functions (p. 630 Sze)
•
MTTF is a common measure of reliability
MTTF =
0
t f(t) dt
•
It is desirable to have a single mathematical model that represents the
failure rate of devices over their entire lifetime
•
(t) generally varies as a function of time as shown
A. High “early failures” or
“Infant Mortality” due to
manufacturing defects
B. “Midlife” or “Steady state”
period of low and generally
constant failure rate
C. “Final” or “wear out”
period
t
C
18
Exponential Distribution Function
•
The simplest distribution function, exponential, is characterized by a
constant failure rate over the lifetime of the device. This is useful for
representing a device in which all early failure mechanisms have been
eliminated
–
(t) =
0
–
R(t) = exp(

0
t)
–
F(t) = 1

exp(

0
t)
–
f(t) =
0
exp(

0
t)
–
MTTF =
0
t
0
exp(

0
t) dt
19
Weibull Distribution
•
(
t) varies as a power of the age of the device
= (
/
)t

1
where
and
are constants
•
For
< 1 the failure rate decreases with time and can be used to represent
early failure
•
For
= 1,
(t) is constant and can be used
to represent
steady state
•
For
> 1,
(t) increases with time and can be used
represent wearout
condition
•
For
= 1, the failure rate is constant which is a special case of Weibull
distribution
•
R(t) = exp{

(1/
)t
}
f(t) =
(
/
) t

1
exp {

(1/
)t
}
MTTF =
1/
(1+1/
) where
=1.
which is linear. The
slope of the line is
. The MTTF is the
time when F(t) = 0.5
ln
ln
)
(
1
1
ln
ln
1
exp
)
(
1
t
t
F
t
t
F
20
In some applications, a better fit can be obtained through the
introduction of a 3rd parameter,
, in which X = t

is used to replace
t in the above equations to represent
•
a shift by the amount of
in the time axis
•
Physically this represents a portion of device lifetime is used up during
manufacturing burn

in or device testing
Accelerated Testing
•
If the required failure rate is
~ 100 FIT or less, then the time required
to observe one failure in 100 devices is approximately 100,000 hr
(11.4 yrs)
•
Thus it is impossible to test the required reliability under normal
operating conditions
•
This necessitates means to accelerate the mechanisms that cause
devices to fail
21
•
5
common stresses are used to accelerate device failure
–
temperature
–
voltage
–
current
–
temperature cycling to accelerate mechanical failure of chips and
assembly package
•
In such studies, different failure mechanisms may be accelerated by
different level of stress even for the same type of stress
•
A device may fail at normal operating conditions because of 2 completely
different mechanisms
•
Under the applied stress, one of these failure modes may be accelerated
much more than the other
•
Thus, we only see 1 failure mode in those tests
•
After successfully eliminating the mode we may only the failure rate by
small factor under normal operating condition
•
Adequate studies must be done under normal operating conditions to
satisfy that no failure mechanism remain that were not accelerated by the
applied stress
22
Temperature Acceleration
•
Many failure mechanisms involve chemical or physical processes that can
be accelerated by raising the temperature
•
E
a
is the activation energy
•
If some parameter of IC changes as a function of time, and if the IC fails
when the parameter exceeds certain value.
•
The Rates at two different temperatures are related as
•
The IC would fail when the destruction reaction proceeds to some value
equal to the failure criterion
•
R
t
f
= constant
•
Thus a plot of ln(MTTF) versus 1/T, the slope will correspond to the
activation energy
)
/
exp(
0
T
k
E
R
R
B
a
2
1
1
2
2
1
1
1
exp
T
T
k
E
R
R
t
t
B
a
)
/
exp(
0
T
k
E
t
t
B
a
f
f
23
Voltage and Current Acceleration
•
Voltage and current are effective acceleration stresses
•
Voltage stress cause failure in devices due to:
–
dielectric breakdown
–
interface charge accumulation
–
charge injection
–
corrosion
•
Most studies indicate that the reaction rate, R
x
, of the failure mechanism is
proportional to a power of the applied voltage
•
where R
0
(T) if thermally activated
•
varies between 1 to 4.5
•
For dielectric breakdown, a different type of acceleration occurs
•
For a given field, a certain fraction of devices fail in a very short time, of
the order of seconds
•
Very few additional failure occurs as the field is maintained
•
If the applied field is increased, additional fraction failures occur
)
(
0
)
(
)
,
(
T
V
T
R
V
T
R
24
•
In such cases, operation at an increased voltage is more in the nature of
screening rather than accelerating the failure mechanism
•
Increased current level is used to accelerate failures caused by
electromigration in metallic conductors
•
1 <
< 4
Stress

Dependent Activation Energy
•
(
T) describes the temperature dependence of the reaction rate
•
For failure accelerated by voltage or current stressing, the activation
energy is dependent on the applied bias
•
The Eyring model states that
•
where S = applied stress
)
(
0
T
J
R
R
T
k
Q
T
k
S
T
a
R
B
B
exp
)
(
sinh
)
(
)
(
)
(
1
0
T
k
T
k
T
T
k
T
a
B
B
B
25
•
Q is related to the Arrhenius activation energy
•
S
B
is the breakdown stress, the value of the applied stress where failure
of the device occurs essentially instantaneously
•
The reaction rate can also be expressed as
•
under conditions of low stress, R reduces to
•
At high stresses
•
From the above expressions Reaction Rate is a function of the applied
stress, the effective activation energy will decrease with increased rate
B
a
S
T
a
E
Q
)
(
0
)
exp(
exp
]
)
(
sinh[
0
1
0
B
B
B
a
S
T
k
S
E
S
T
R
)
exp(
exp
)
(
0
1
0
B
B
B
a
S
T
k
S
E
S
T
R
T
k
S
S
E
S
S
R
B
B
a
B
1
1
0
0
exp
)]
(
exp[
26
Humidity

Temperature Acceleration
•
Presence of water vapor in the chip environment introduces a new variety
of possible failure mechanism
•
Water vapor quickly permeates plastic packaging material
–
1. water vapor transports contaminants from surface of package
through the plastic
–
The chip is then exposed to water vapor and various contaminants
–
2. Diffusion of the contaminated water vapor through the passivation
layer of the chip
–
This step can be speeded up if the passivation contains defects or
cracks
–
The penetration of water vapor through the passivation layer
determined the reaction rate
–
3. Once water reaches the metallization level, electro

chemical
corrosion process can occur
–
The ions needed for this corrosion process can arise from the
contaminants which diffused through the passivation layer.
27
–
If the intermediate dielectric of the chip is a phosphorous

doped
glass, the water vapor can extract the phosphorus from the
dielectric
–
Electrochemical corrosion is a rapid process leading to
metallization failure
–
This failure mechanism can be accelerated by increasing the partial
pressure of water vapor in the environment
28
Burn

in
•
For mature products, the initial reliability studies would have identified
and eliminated failure processes so that steady

state failure rate meets
or exceeds design goal
•
However, the manufactured devices still show existence of continuing
early failure
•
Generally, manufacturing defects cause the infant mortality failures
e.g. pinholes, photoresist or etching defects resulting in near

opens or
shorts
•
Contamination on the chip of the package, scratches, weak chips or
wire bonds, partially cracked chips or packages
•
The purpose of the burn

in procedure is to operate the devices for
some time during which most of the devices that are subject to
•
Infant mortality failure actually fail
•
The conditions during burn

in presumably accelerate the failure
mechanisms that contribute to infant mortality failure
•
Studies of infant mortality under increased T conditions show that
infant mortality have an activation energy of 0.37 to 0.42 eV
29
Properties of Metal

Oxide Silicon (MOS) System
•
To understand the MOS system the step is to derive the energy band
diagram
•
We note that at thermal equilibrium the Fermi level is constant
•
The energy band diagram for a separated system is shown below:
E
0
E
fm
q
M
= 4.1 eV
E
C
E
V
8 eV
E
C
E
V
E
fs
E
i
= 4.1 eV
q
30
•
When connected the Fermi
level will be constant. The
Fermi level in Si depends on
doping level of the Si
•
For E
i

E
f
= 0.29 eV the band
diagram is shown
E
fm
C
i
V
fs
E
E
E
E
Accumulation
E
fm
C
i
V
fs
E
E
E
E
Flatband Condition
31
E
fm
C
E
fs
E
i
E
V
E
Weak Inversion
E
fm
C
E
fs
E
i
E
V
E
Depletion
E
fm
C
E
fs
E
i
E
V
E
Strong Inversion
q
p
q
s
32
•
Strong inversion condition stipulates that q
P
=
q
s
•
Thus to turn an MOS into strong inversion

a condition for the
formation of a conduction channel or inversion layer under the gate, a
minimum band bending of 2
q
P
is required
•
The threshold voltage V
T
is then represented by
•
We can gain further insight into the MOS by realizing that it is
basically a capacitor
•
The charges in the Si of the MOS system can be expressed as
•
The terms in the square brackets constitute the voltage drop across the
oxide. Since part of the charges are associated with the dopants in the
depletion layer, therefore free carrier concentration in the inversion
layer is


4
1


2
p
A
s
ox
p
FB
T
qN
C
V
V
)]
(
)
[(
p
s
FB
G
ox
V
V
C
Q


4
)

2
(
P
A
S
p
FB
G
ox
n
N
V
V
C
Q
33
•
The second term is the charge in the depletion layer V
G
here is the gate
bias required to produce a band bending of 2
P
 and is therefore
equivalent to the threshold voltage
•
The proof for the expression of charge in Si is
s
d
A
x
qN
34
•
Where E is the electric field in Si
•
The total band bending in Si is
•
From Poisson’s equation we have
•
For x
d
= x
dmax
we have
s
= 2
p
and
•
Charge is the Si layer is qN
A
x
dmax
, thus
•
The total charging voltage is
•
where
d
s
x
E
0


s
d
A
s
x
qN
2


A
p
d
qN
x
4
max
p
A
d
qN
Q
4
si
ox
V
V
V
p
s
si
V
)
(
p
s
ox
FB
G
V
V
V
ox
ox
ox
s
ox
ox
s
ox
p
s
FB
G
ox
ox
ox
x
C
E
E
x
V
V
x
V
E
'
)]
(
)
[(
35
•
Substituting into the previous equation
•
From Poisson’s equation we obtain
•
Concentration of free carriers in the inversion layer is
Oxide and Interface Charges
•
Charges at Si

SiO
2
interface and the oxide may influence the threshold
voltage through the modifications of the flat

band voltage. If the density
of charge at x=x
1
. It induces an equal and opposite charges divided
between silicon of the metal gate. The closer is x1 to x
ox
(the Si

SiO
2
interface), the greater will the fraction of induced charges at Si

SiO
2
interface and the oxide may influence the threshold voltage through the
modifications of the flat

band voltage. If the density of charge at x=x
1
. It
induces an equal and opposite charges divided between silicon of the metal
gate. The closer is x
1
to x
ox
(the Si

SiO
2
interface), the greater will the
fraction of induced charge within the Si.
•
The induced charge changes the charge stored in the Si at equilibrium
therefore it alters the flatband voltage.
•
The size of
V
FB
can be found using Gauss’ law to obtain the value of the
gate voltage that causes all of the oxide charge Q
ox
to be mirrored in the
gate electrode.
)
(
)
[(
'
p
s
FB
G
ox
s
s
V
V
C
E
'
'
'
d
n
s
s
Q
Q
Q
E
)
(
'
T
G
ox
n
V
V
C
Q
36
•
Under this condition the field is constant between x = 0 and x =x
1
and
0 for x > x
1
.
•
For 0 < x < x
1
we have the following relationship
•
The result can be generalized to account for shift in VFB using an
arbitrary charge distribution
•
where
(x) is the volume charge density at x
Origins of Oxide Charges
•
There are at least 4 distinct types of charges in the oxide

silicon system
–
Q
f
’

fixed interface charge density
–
Q
ot
’

oxide trapped charge density
–
Q
it
’

interface trapped charge density
–
Q
m
’

mobile charge density
1
'
0
,
x
x
Q
E
ox
ox
ox
'
'
1
ox
ox
ox
FB
C
Q
x
x
V
dx
x
x
x
C
V
ox
x
ox
ox
FB
)
(
1
0
'
37
•
Q
f
’ is positive and is located within a very thin (1

2nm) laryer fo non

stoichiometric silicon oxide (SiO
x
)
•
Q
ot
’ can be both positive and negative, typically predominantly
negative. Located in traps distributed throughout the oxide layer.
Distortion in the C

V curve is due to unstable charges at the interface.
•
The trapping sites N
it
(cm

2
) are located at the Si

SiO
2
interface and
have energy levels within the bandgap with density D
it
cm

2
eV

1
•
To relate behavior of these traps to the distorted C

V
G
, as shown in the
following figure, consider an oxide

Si interface characterized by
interface trapping levels at energy E
s
. The gate voltage causes the
Fermi level at the surface to cross E
s
, the charge state of these levels
will change. This introduces a voltage dependent term, Q’it/Cox’, into
the equation for V
FB
above making both flatband and threshold
voltages vary with VG that led to the distortion the C

V curve.
•
For N
it
> 10
10
cm

2
is generally unacceptable for reliable device design.
Using modern MOS technology, N
it
is reduced by annealing device in
forming gas (90% N
2
and 10% H
2
)
38
Mobile charge results from alkali

metal ions particularly sodium.
They induce
V
FB
.
•
The alkali ions have sufficient mobility when relatively low gate biases
are applied. The mobility increases with temperature and thus
magnifies the problem of VFB instability at high temperatures. The
ions are positively charged, therefore

V
G
draws the ions to the metal

SiO
2
intrface where their effect is minimal. +V
G
pushes them to the
Si

SiO
2
interface where their effects are most significant.
•
For voltage stability of 0.1V, less than 2x10
10
cm

2
mobile ions can be
tolerated. Mobile ions can be avoided by careful processing and
oxidation in HCl that immobilizes alkali ions.
Hot Electron Degradation
•
The assessment and improvement of reliability on the CKT level
should be based on both failure mode analysis and the basic
understanding of the physical failure mechanisms.
•
Processes such as electromigration and electrostatic discharge cause
catastrophic changes in device characteristics
39
•
Other mechanisms such as hot

electron effects cause non

catastrophic
failures which develop gradually over time and change CKT
performance
Scattering of Channel Hot

Electrons into the Oxide
•
In order for electrons to obtain enough kinetic energy to be injected
into the oxide, it has to
–
gain K.E.
–
its momentum redirected towards the oxide through a quasi

elastic
collision
–
following the collision, the electron must travel to S

SiO
2
without
further collision
•
These processes are statistically independent, the injection probability
is obtained as the product of the probabilities of each event
•
MOSFET gate current is made up of electrons injected into the gate
oxide by quasi

elastic scattering
•
It consists of electrons that overcome the image potential well in the
oxide and reach the gate electrode
40
Hot Carrier Effects
•
Advances in VLSI is achieved through down scaling of device
dimension such as channel length, junction depth and gate oxide
thickness without proportional scaling of power supply voltage
•
Decrease in device dimensions results in significant increase of the
horizontal and vertical electric fields in the channel region
•
Electrons or holes with high K.E. may be injected into the gate oxide,
degrading I

V characteristics of MOSFETs.
•
This is one of the important factors that limits the maximum
achievable device densities in VLSI circuits
•
Hot

carrier damage results in:
–
trapping of carriers on defect sites in the oxide
–
creation of interface states at Si

SiO
2
interface leads to degradation
in transconductance, shifts in threshold voltage and decrease in
drain current capability.
41
Oxide degradation Mechanism in MOS system
•
Cause by injection of high

energy electrons and holes into the gate
oxide near the drain
•
The damage is in the form of localized oxide charge

trapping and
interface trap generation
•
Recent experimental evidence shows that hot

carrier related
degradation can occur in deep

submicron devices with L
eff
= 0.15
m
at drain voltage as low as 1.8V. Therefore hot electron degradation
may occur even with significant reduction in drain voltage.
•
The continuing technology thrust must therefore accompanied by some
limitations to ensure hot

electron reliability
•
Hot

carrier injection causes degradation in the transconductance, shift
in threshold and decrease in sub

threshold drain current
•
There are many disagreement concerning the physical degradation
mechanisms due to the lack of a reliable and sensitive techniuqe to
evaluate hot

carrier damage at the interface. Moreover, hot

carrier
induced oxide damage is very localized, the interpretation of the
analysis is complex
42
Injection of Hot

Carriers into Gate Oxide
•
Hot

carriers are electrons and holes that have a much higher K.E. than
average carrier population
•
E’s in S.C. at equilibrium mostly have energy about k
BT
above E
C
. At
equilibrium, K.E. of carriers that encounter large may gain
significant K.E. in a short distance. Thus E

E
C
= k
B
T
e
where T
e
is the
effective electron temperature. There are 2 distinct modes of electrons
injection in nMOS
–
Substrate hot

electron effect (SHE)
–
Channel hot

electron effect (CHE)
•
Substrate hot

electrons are derived from leakage current. Electrons
generated in the channel depletion region or diffusing from the bulk
neutral region of the substrate drift toward the Si

SiO2 interface and
gain K.E. from the high field in the surface depletion region
•
The energetic electrons may overcome surface energy barrier and
inject into the gate oxide.
•
Some of the injected electrons are trapped in the oxide, resulting in a
relatively uniform oxide charge accumulation that shifts the threshold
voltage over time.
E
43
•
The SHE is observed mainly in long

channel MOSFETs. As channel
length decreases, SHE decreases since a large fraction of the hot

electrons generated in the substrate region are swept into the source
and drain regions instead of the device surface
•
CHE is more pronounced at large V
DS
. Electrons reaching Si

SiO
2
interface with large K.E. may surmount the energy barrier. Electrons
and holes generated by impact ionization also contribute to charge
injection into the oxide. Hot

electron current and oxide degradation
occurs mainly at the drain end. From the figures, the increased density
of equipotential lines leads to larger horizontal field. Hot

electrons
and hot

holes can be injected into the oxide interface with the aid of
the vertical field or with their K.E. energy alone.
•
Injected current density is
•
Where n(x,y) is the local electron concentration at (x,y)
•
p
inj
(x,y) is the spatial distribution of injection probability
•
p
inj
(x,y) depends on several events that provide the electron with a
momentum directed towards the oxide interface and with a K.E.
sufficient to overcome interface potential barrier.
y
inj
e
dy
y
x
p
y
x
n
x
J
)
,
(
)
,
(
)
(
44
•
Injection of hot carriers occurs mainly in a narrow injection zone at the
drain end of the device where lateral field reaches maximum.
•
In log channel MOSFETs, the spatial extent of injection region and
magnitude of electric fields near the drain are largely independent of
the channel length, L.
•
For short channel devices, the heavier dopin or shallower junctions
increase the electric fields in the drain region. Due to short channel
effects the channel current entering the drain increases more rapidly
than 1/L.
•
Thus, devices with smaller geometries will be more sensitive to hot

carrier related degradation.
•
Oxide degradation in the form of charge trapping which occurs in a
short distance of about 0.1
m. However, a large percentage of the
electrons entering the oxide are either scattered in the oxide and/or
returned to Si substrate by the opposing field.
•
The charges that do not reach the gate electrode degrades the oxide by
charge
trapping and interface trap generation.
45
Impact Ionization by Hot

Electrons
•
In saturation region a high exists in the channel depletion region.
Electrons will, therefore, be accelerated by the field. Some move
horizontally and creates electron hole pairs (EHP) by impact ionization
near the drain.
•
Impact ionization process creates an avalanche plasma consisting of
generated EHP in the pinch

off region
•
The holes created are collected by the substrate constituting the drift
component of the substrate current
•
The drain current that contributes to impact ionization substrate current
is a function of lateral electric field in pinch off region and V
GS
and L
E
Impact
Ionization
46
•
Some electrons and holes in the avalanche plasma can gain sufficient
K.E. to surmount Si

SiO
2
potential barrier and become injected into
SiO
2
. Majority of the holes generated constitute substrate current of
MOSFET. Therefore, substrate current is considered a reliable and
convenient monitor of the amount of hot

carrier degradation in n

MOSFETs
•
To create EHP, hot

electrons must have K.E. > (impact ionization
energy). Thus is the distance the electrons must travel in
to gain energy
i
.
•
The probability of an electron travelling a distance to gain the required
K.E. or more is
where
is hot

electron mean

free path. Since IDS is the total electron
flow in the channel. Rate of supply of hot

electrons with K.E. >
i
is
where C
1
is a weak function of the max. channel field E
m
.
i
m
i
E
q
/
m
E
E
]
exp[
m
i
i
E
q
P
)
exp(
1
m
i
DS
sub
E
q
I
C
I
47
Oxide Traps and Charge Trapping
•
Concentration of oxide trapped charges and interface trapped charges
are changed by capture of excess electrons or holes by existing traps in
the oxide.
•
The oxide charge distribution can also be changed by impact release of
the trapped electron or hole by a hot

carrier. The electron or hole traps
in the gate oxide are mainly Si “dangling bonds”. The dangling bonds
give rise to the electron and hole traps.
Interface Trap Concentration
•
Interface trapped charge arises from a.) structural, oxidation

induced
defects; b.) metal impurities; c.) defects caused by radiation or hot

carriers
•
Unlike other trapped charges, interface trapped charges are in electrical
communication with the underlying Si. Thus, influence of interface
trapped charge on electrical characteristics of MOSFETs depends on
its bias conditions.
•
Generation of new interface trap is the primary cause of degradation of
MOSFETs. New traps generated by hot

electrons and hot

holes
through breaking:
48
–
Si

Si and Si

O bonds
–
breaking of H bonds at interface, releasing H and leaving dangling
Si

or O

bonds
–
H released by hot

carrier impact migrates towards Si

SiO
2
interface and is then trapped by proton traps.
Bias Dependence of Degradation Mechanism
•
Oxide degradation takes place by carrier trapping in oxide due to hot

electron carrier injection and interface trap creation
•
These are the two most significant degradation mechanism, but there is
no clear consensus on their relative contribution Hot

carrier related
device degradation reaches maximum when VGS = VDS/2. This
coincides with max. of substrate current, thus it is often linked to
impact ionization.
•
When VTH shift is plotted as a function of gate voltage, the
degradation exhibits 2 local maxima:
–
First peak: electron injection into SiO2 is max. resulting in charge
trapping
–
Second peak: at VGS = VDS/2, corresponds to impact ionization
of electrons and holes.
49
•
For V
TH
= V
DS
/2,
V
TH
(t) = At
n
where 0.5 < n < 0.7
•
A depends on I
SUB
, I
DS
and processing parameters
Effects of Hot

Carrier Damage on Device Characteristics
•
Trapped charges in gate oxide influence surface potential and thus
local flat band voltage
•
C

V measurement can be used to measure total amount of trapped
charge in SiO
2
. Accumulating negative charge shifts the local VFB to
positive direction.
•
Influence of interface traps generated by hot

carriers depends on the
instantaneous bias conditions. Since interface traps are in electrical
communication with the underlying Si substrate, occupation of the
traps depends on the Fermi level at the Si

SiO
2
intface and energy
distribution of interface traps and the physical nature of N
iT
(whether
the trap is acceptor or donor type).
•
In n

MOS most generated N
iT
are acceptor type, mostly located at the
drain end. Traps
will start to be charged by electrons from substrate as
the surface is biased from accumulation into weak inversion, ant then
into strong inversion
50
•
Once all traps are filled, their influence is similar to fixed oxide
charge, which is the case because for all practical purposed the
device are in strong inversion
•
Surface mobility is decreased due to increased surface scattering
•
Significant reduction in I
D
in linear region
•
Less effect on I
D
in saturation region because once in saturation I
D
is governed by the channel region between the source and pinch off point
•
Asymmetry between forward and reverse I

V curves also due to
localization of oxide damage near the drain end
–
as
n
decreases g
m
decreases
–
I
D
/I
D0
decreases
–
V
T
increases
Radiation Induced Interface Traps
•
The major effect of ionization radiation on MOS devices is the
generation of positive oxide charge resulting from hole

trapping at Si

SiO
2
interface.
51
•
Radiation consists of high energy particle such as electrons, neutrons,
protons and energetic x

ray and gamma ray
•
Photons with E > E
G
of SiO
2
can generate EHP. Some of the
generated carriers recombine. Most are driven toward the electrode by
the oxide field. Electrons rapidly drift toward the positive electrode
and flow out of the circuit. Holes drift much more slowly towards
negative electrode.
•
Once holes reach Si

SiO
2
interface a fraction becomes trapped
constituting the radiation induced positive oxide charge
52
Latchup in CMOS Circuits
•
CMOS (Complementary MOS) is a very important class of circuits in
VLSI technology
•
Advantages of CMOS circuits includes low power, high speed logic
circuits
•
In bulk CMOS CKTs both n

and p

channel MOSFETs exist side by
side. This is achieved by starting with a Si wafer of one type and
creating in it regions of the opposite type. In so doing, FETs are not the
only structures fabricated, pnpn devices consisting of parasitic bipolar
transistors are also created.
V
DD
V
o
i
V
PMOS
NMOS
V
DD
V
o
V
ia
V
ib
53
•
Under normal operation the circuit performs as an inverter and the
bipolar portion can be ignored. However, if the bipolar circuit
switches from its normally high impedance state to its low impedance
state, the power supply sees a low impedance path to ground.
•
If the current from the supply is not limited somehow, there might be
irreversible damages done to the circuit.
•
However, even if the circuit is protected, the pnpn’s low impedance
state can still cause the circuit to malfunction.
54
Switching Mechanism (Streetman p. 401)
•
The operation of a CMOS
circuit can be understood using
a two

transistor analogy
p
n
p
n
n
p
i
E
B
C
C
B
E
1
2
b
c
=
i
1
i
1
=
c
i
2
b
i
2
J
1
3
J
2
J
2
J
1
1
2
2
2
1
•
Thus the parasitic bipolar transistors in a CMOS inverter can be
viewed has two interconnected BJTs
•
Each BJT can be modeled by Ebers Moll model
S
N
n
E
C
P
P
S
E
P
P
E
B
I
CS
C
P
n
P
n
CS
C
P
P
n
55
•
The Ebers

Moll model uses the diode equations for the emitter and
collector plus extra terms that provide coupling between the emitter
and collector.
•
For a forward biased diode, the excess carriers is
•
Thus the emitter current is
•
Thus, IC and IE can be expressed as
)
1
(
/
T
k
qV
n
E
B
e
p
p
)
(
C
N
E
n
ES
n
C
CS
I
n
E
ES
E
p
p
p
I
p
p
I
p
p
I
I
)
(
C
E
I
n
CS
n
C
CS
n
E
ES
N
C
p
p
p
I
p
p
I
p
p
I
I
)
1
(
)
1
(
)
1
(
)
1
(
)
1
(
)
1
(
/
0
/
/
0
/
T
k
qV
E
C
I
E
T
k
qV
ES
I
N
C
I
E
T
k
qV
C
E
N
C
T
k
qV
CS
I
N
E
N
C
B
EB
B
EB
B
CB
B
CB
e
I
I
I
e
I
I
I
e
I
I
I
e
I
I
I
56
Two

Transistor Analogy
•
The analysis of the 2

transistor analogy is given below:
•
where
1,2
are the emitter

to

collector current transfer ratios for the
transistors
•
However, the sum of
i
c1
and
i
c2
is the total current through the device.
Thus,
•
As indicated in the above equations, as long as the sum,
1
+
2
, is small
compared to unity,
the current i is small at approximately the combined
collector saturation currents of the 2 equivalent transistors
. As
1
+
2
approaches unity the current i increases rapidly. At this state both
transistors become saturated and will remain in the low resistance state
after the switching.
1
02
2
2
2
01
1
1
b
C
c
b
C
c
i
I
i
i
i
I
i
i
)
(
1
)
(
2
1
02
01
02
01
2
1
2
1
C
C
C
C
c
c
I
I
i
i
I
I
i
i
i
i
57
Variation of
w楴栠䥮橥瑩潮
•
Since the 2

transistor analogy implies that switching involves an
increase in the
1
and
2
to the point that
1
+
2
becomes unity, it is
important to understand how
1
and
2
depend on injection for a
transistor.
•
is the product of the emitter injection efficiency,
, and the base
transport factor, B where
•
At very low currents,
is dominated by
recombination in the transition
region of the emitter junction
•
As the current increases, injection across the junction begins to
dominate over the recombination. This leads to increase in
B due to
the saturation of recombination centers as excess carrier concentration
becomes large.
En
C
Bp
En
En
I
I
B
I
I
I
;
58
Forward Blocking State
•
At this state the applied voltage is mainly across the reverse biased
junction j
2
•
j
1
and j
3
are forward biased but current remain small because holes are
injected from p
1
into n
1
.
•
If a hole recombines with an electron in n
1
the electron must be
replenished to maintain space charge neutrality.
•
The supply of electrons is very restricted because j
2
is reverse biased.
•
As a result current through j
1
is approximately the same as the reverse
saturation current of j
2
. Similar arguments hold for current through j
3
.
59
Conducting State
•
As
1
+
2
1, many holes injected at J
1
survive to be swept across j
2
into p
2
. Similarly, electrons injected at j
3
are collected at j
2
. This is
regenerative because more electrons injected into n
1
induces more holes
injection across j
1
to maintain neutrality.
•
When this happens depletion at j
2
begins to shrink. Finally, j
2
becomes
forward biased.
•
The overall voltage across the devices approximates the potential drop
across 1 forward biased pn junction.
•
The triggering of the junction is often caused by the breakdown of j
2
60
Avoiding Latchup
•
Latchup can be avoided by incorporating guard structures in the circuits.
•
There are two types of guard structures
–
minority carrier guards
–
majority carrier guards
•
The guard structures are used to decouple the parasitic bipolar transistors
from each other
Minority Guard
•
Minority carrier guards are used to collect injected minority carriers
before they can cause a problem.
•
The minority carriers injected into the substrate could be collected by a
reversed

biased well/substrate junction and flow through the well as
majority carriers.
Majority Guard
•
The basic mechanism of a N
+
majority guard ring in the well is to steer
current away from the parasitic emitter.
61
Silicon on Insulator (SOI)
•
Devices fabricated on SOI substrates are fabricated by dielectric
separation
•
At this point the most mature technology for manufacturing SOI
substrates is Separation by IMplantation of OXygen (SIMOX)
•
In this technology heavy dosage of oxygen is implanted into Si wafer
to obtain SiO
2
with a layer of single crystalline Si on top
•
Separation of devices can therefore be accomplished by etching the Si
layer through
•
Therefore there will not be any parasitic bipolar transistors
Enter the password to open this PDF file:
File name:

File size:

Title:

Author:

Subject:

Keywords:

Creation Date:

Modification Date:

Creator:

PDF Producer:

PDF Version:

Page Count:

Preparing document for printing…
0%
Comments 0
Log in to post a comment